Dottorato di ricerca in Scienza e Tecnologia dei Materiali Innovativi
Ciclo XXVIII (2013-2015)
Self-standing curved crystals for X and Gamma ray focusing
Prof. Enrico Dalcanale Tutor:
Dott. Claudio Ferrari Dott.ssa Elisa Buffagni
Dottorando: Elisa Bonnini
1 Laue Lens Concept 5
1.1 Astronomical application . . . 7
1.2 Medical application . . . 9
2 Diraction of X and g ray from crystals 13 2.1 Fundamentals of crystallography . . . 13
2.1.1 Crystalline structure . . . 13
2.1.2 Reciprocal lattice . . . 15
2.1.3 Diraction condition: Bragg and Laue relation . . . 16
2.1.4 Ewald construction . . . 18
2.1.5 Geometries of diraction . . . 19
2.2 Diraction from ideal crystal . . . 19
2.2.1 Thomson scattering from a free electron . . . 19
2.2.2 Scattering from an atom . . . 21
2.2.3 Diracted intensity from a small single crystal . . . 23
188.8.131.52 Integrated intensity from small single crystal . . 24
2.2.4 Limitations and corrections to the kinematical theory: the dynamical theory . . . 25
2.2.5 The dispersion surface . . . 26
184.108.40.206 Qualitative approach to the dynamical theory . . 27
2.2.6 Integrated Intensity and reectivity in Laue case in dy- namical theory . . . 30
2.2.7 Borrmann eect . . . 35
220.127.116.11 Polarization inuence . . . 35
2.3 Diraction from mosaic crystal . . . 36
2.3.1 Darwin model . . . 36
2.4 Diraction from crystal with curved diracting planes . . . 38
3 Diraction eciency of bent crystals: theoretical study 43
3.1 Diraction eciency . . . 44
3.1.1 Approximated calculation of integrated intensity: Lamel- lar model . . . 45
3.1.2 Crystal's material . . . 46
3.1.3 Eect of crystal's thickness . . . 46
3.1.4 Radius of curvature . . . 49
3.2 Conclusion . . . 50
4 Bending technique 53 4.1 Damaging technique . . . 54
4.2 Resin deposition technique . . . 56
4.3 Conclusion . . . 60
5 Experimental results 65 5.1 Low energy . . . 65
5.1.1 Preparation of thicker diracting elements . . . 70
5.2 High energy . . . 73
5.3 Conclusion . . . 75
6 LAUE Project 79 6.1 Crystal selection . . . 80
6.2 The Larix facilities . . . 82
6.2.1 Alignment of the facility . . . 86
6.3 Focusing eect . . . 88
6.4 Conclusion . . . 92
Conclusions 99 A Calculation of the inner lattice plane bending in bent crystals101 B Origin of strain in surface damaged bent crystals 105 B.1 Line tension characterization . . . 105
B.2 Model of strain formation in surface treated crystals . . . 107
B.3 Mechanism of dislocation formation . . . 108
C Experimental set up 111 C.1 ANKA Synchrotron radiation facility . . . 111
C.2 Hard X ray Facility, ILL . . . 113
The focusing of hard X and g rays in the energy range between 60 and 600 keV has important applications in astronomy to improve the sensitivity of telescopes (Frontera et al., 2005) and in nuclear medicine for in vivo diagnosis of diseases associated with organ malfunctioning, for cancer detection (Roa et al., 2005) and for focussed radiotherapy. A clear example is given by the case of scinti- graphic monitoring, in which target images are currently obtained by collecting monochromatic g radiation coming from specic radiopharmaceuticals, selected in the emission energy range from 80 keV (Xenon-133) to 511 keV (Fluorine-18), by means of gamma cameras based on ne multi-hole collimators and scintil- lators. A major drawback in such systems is the high dose distributed to the body because most of the radiation is lost by collimator absorption.
Bragg diraction in Laue geometry is a method to focus high energy X and g rays. This is the goal of a Laue lens, which is composed of a set of crystals disposed in concentric rings and properly oriented in order to concentrate the diracted beams into a small focal point on the detector (see Chap. 1).
Crystals suitable for such a lens should be able to eciently diract the radiation in an angular range from a few tens of arc seconds up to some minutes of arcseconds, depending on the required lens resolution. Perfect crystals cannot be used due to their very narrow angular range of diraction at g ray energies.
Instead, mosaic crystals are good candidates as optical elements for these lenses, because their angular acceptance can be directly tuned by modifying the mosaic spread and/or the size of microcrystals forming the mosaic structure during the growth process. Mosaic crystals of high diraction eciency at g ray energies, such as Cu, Au, Ag and many others, have been proposed (Lund, 1992; Courtois et al., 2005; Barriere et al., 2009) due to their high electronic density and structure factor. Moreover, the integrated intensity Iint (dened as the area of the diraction prole for a monochromatic radiation, which gives directly an indication of the diraction eciency of the crystal) of an ideal mosaic crystal can be two orders of magnitude larger than that of a perfect crystal, as predicted by the dynamical theory of X ray diraction (Authier, 1998). Unfortunately the production of crystals with well-dened mosaic spread and grain size is a dicult technological task, so that the resulting diracted intensity is often
much lower than that predicted for the ideal case. Mosaic crystals of high diraction eciency at g ray energies, such as Cu, Au, Ag and many others, have been proposed (Lund, 1992; Courtois et al., 2005; Barriere et al., 2009) due to their high electronic density and structure factor.
An eective alternative is represented by self-standing bent crystals, in which the external curvature induces also a bending of the diracting planes.
In this case the Bragg condition is satised for a broad angular range accord- ing to the degree of curvature; this also causes the high angular acceptance of these crystals (Smither et al., 2005). If the curvature radius R is smaller than a critical value resulting from dynamical theory, curved diracting plane (CDP) crystals can theoretically reach the Iint values obtained for ideal mosaic crystals (Malgrange, 2002).
In this thesis a theoretical study of the Iint of CDP crystals is presented in Chap. 3, based on dynamical theory of X and g ray diraction, described in Chap. 2. The theoretical study point out what are the best material and values for parameters, such as thickness, curvature, dimensions, and diraction geometry to maximize the diraction eciency of curved crystals in the energy range of interest.
In Chap. 4, two dierent simple methods to obtain self-standing curved crystals with reproducible and uniform curvature are presented. The rst one is based on the controlled surface damaging induced by a mechanical lapping process (Buagni et al., 2011). A compressive strained layer of few micrometres in thickness is generated and causes the convex curvature of the damaged side of the crystal (Buagni et al., 2012; Buagni et al., 2013). This technique allows to obtain external radii of curvature R down to 2 m in crystals with thickness up to 2 mm in the direction perpendicular to the damaged surface. The diraction prole of CDPs, parallel to the damaged surface, is close to that of an ideal bent crystal curved by elastic deformation (Ferrari et al., 2014).
Another innovative and simple bending technique presented for the rst time in this work is based on the shrinking of resins during a polymerization process, as it is well known in wood and mechanical industry. The process consists on a lm deposition of selected bi-component epoxy resin on one side of crystals with thickness uniformity guaranteed by means of a spin-coater. During the polymerization, the resin induces a tensile strain that causes the bending of the substrate, with concave curvature on the side of the resin deposition.
In order to verify the theoretical results obtained about the crystal dirac- tion eciency, detailed characterizations at low and high X ray energies are performed on at and bent crystals obtained with the damaging and the resin deposition techniques, Chap. 5. Thanks to the access to the European facili- ties, as ILL and ANKA synchrotron, it was possible to perform a quantitative study of the diraction eciency of crystals with dierent thickness at dierent geometries, in the energy range of interest.
To complete this work, the study of the focusing eect of GaAs curved crystals realized with the damaging tecnique are shown in Chap. 6. The contest is a project founded by the Italian Space Agency (ASI), called LAUE project, that was devoted to create a technology to build a Laue lens with long focal length (f =20 m) able to focus photons in the 70ö300 keV energy range. The lens is assumed to be made of petals constituted by a large number of crystals tiles disposed in concentric rings and properly oriented in order to diract an incident beam parallel to the lens axis in the focal point of the lens. In this case, curved crystals are directly used as focusing optical elements.
Laue Lens Concept
Diraction lenses are based on the interference between the X and g radiation and the periodic structure of matter in a crystal. In a Laue lens, an incoming beam with wavelength l, passing through the whole volume of crystals, can be diracted if it satises the Bragg condition (see sec. 2 ),
2dhklsin θ = nλ (1.0.1)
With dhkl the spacing of a chosen set of planes (hkl). The Bragg condition can occurs in two dierent geometries (reection and transmission), illustrated in Figure 1.0.1 and explained in detail in sec (2.1.3).
Figure 1.0.1: The Bragg condition for constructive interference of an X and g ray with the atoms of a given crystalline plane. (a) Bragg diraction in reection cong- uration (Bragg geometry). (b) Bragg diraction in transmission conguration (Laue geometry), (Frontera and von Ballmoos, 2010)
A Laue lens is made of a large number of crystals disposed in concentric rings (Figure 1.0.2 Left) properly oriented in order to diract, in Laue geometry, the incident radiation into a common focal point (see Figure 1.0.2 Right). The lens has a shape of a spherical cup, with a radius of curvature R, covered with
crystal tiles having their diracting planes perpendicular to the surface of the sphere. The focal spot falls on the detector placed on the lens axis at a distance f = R/2from the cup, where f is called the focal length.
Figure 1.0.2: Left: Scheme of the disposition of crystals in concentric rings on a Laue lens . Right: Concentric rings at a given ring r concentrate a dened energy E into the focal point (Frontera and von Ballmoos, 2010).
Considering the Bragg equation 1.0.1, for the rst diraction order (n = 1);
the energy E of an incident beam diracted by a set of crystals disposed in a ring at distance r (rmin≤ r ≤ rmax) from the lens axis, is:
E = hc
i ≈ hcf
Assuming that chosen diracting planes (hkl) of all the crystals that com- pose the lens are the same; the energy of the photons diracted from all the crystals in the ring will be centered on E. A Laue lens can diract photons over a certain energy passband (Emin, Emax):
(1.0.3) The energy passbands of the diracted photons by contiguous crystal rings have to overlap each other in the focal point.
Suitable crystals must be selected as optical elements for a Laue lens. The angular acceptance α of a perfect crystal, represented as the full width at half maximum (FWHM) of the diracted prole (known as the Darwin width), is extremely narrow (fractions of an arcsec to a few arcsec depending on the photon wavelength, see (Zachariasen, 1945)), whereas angular acceptances of
several tens of hundredth arcsecond are desirable; therefore perfect crystals are not suitable for Laue lenses. In order to increase the angular acceptance or the energy passband of individual crystals, mosaic crystals or curved crystals must be used. For astronomical applications, crystals with mosaicity or total bending angles ranging from a few tens of arcseconds to a few arcminutes are of interest.
The focal length f has a key importance in the case of Laue lenses. Indeed from the expression of the energy passband (Emin, Emax) of a lens, it results that the lens radii (rmin, rmax) depend linearly on f :
(1.0.4) High energy photons are diracted by the inner part of the lens so, to get a lens with a dened inner area, the focal length must be increased. It is important to note that the lens area approximately increases with f2. An X and g ray lens with a broad coverage from 300 keV to 1.5 MeV was proposed by Lund (Lund, 1992, Lund, 2005). He assumed the lens constituted by mosaic crystals of Copper and Gold. In order to achieve a signicant eective area at high energies (350 cm2 at 300 keV and 25 cm2 at 1.3 MeV), the focal length proposed was 60 m.
1.1 Astronomical application
Broad band X and g ray missions, like BeppoSAX, and INTEGRAL, have shown that, in order to better understand the physics underlying several classes of galactic and extra-galactic sources, two main requirements on the instrumen- tation are crucial (Frontera et al., 2012):
1. to be able to cover a broad energy band: from a fraction to several hundred of keV;
2. to achieve a high spectrum sensitivity.
The current experimental scenario is the following:
low energy X ray (0.1ö10 keV) telescopes are available and are well tested in space;
medium energy X ray (up to 70/80 keV) telescopes, based on multilayer mirrors, are mature and will be tested in space in the next future;
high energy X ray (>70/100 keV) telescopes are under development.
To take full advantage of the extraordinary potential of hard X and soft g ray astronomy, a new generation of focusing telescopes is needed.
With Laue lenses, a big leap in both ux sensitivity and angular resolution is expected. In particular, for the sensitivity the expected increase is by a factor of 10 100 with respect to the best non-focusing instruments of the current generation. Concerning the angular resolution, the increase is expected to be more than a factor 10 (from ∼15 arcmin of the telescopes like INTEGRAL IBIS to less than 1 arcmin), (Frontera and von Ballmoos, 2010).
The astrophysical issues that are expected to be solved with the advent of these telescopes are many and of fundamental importance. A thorough dis- cussion of the science case has been carried out in the context of the mission proposal Gamma Ray Imager (GRI), submitted to ESA in response to the rst AO of the Cosmic Vision 20152025 plan (Knödlseder et al., 2009; Frontera et al., 2005; Knödlseder, 2006).
Some of these astrophysical issues are:
I. Deep study of high energy emission physics in the presence of super- strong magnetic elds (magnetars); soft Gamma Ray Repeaters (SGRs) and Anomalous X ray Pulsars (AXPs) have raised many questions related to the role of their strong magnetic eld in the high energy emission (> 100 keV). Furthermore, also the belonging of these two types of source to the same class can be understood.
II. Deep study of high-energy emission physics in compact galactic ob- jects and Active Galactic Nucleus (AGNs); high energy emission in compact galactic objects and AGNs is also not well understood. The emission region can be investigated measuring the high energy cuto
and its relation to the power-law photon index of the energy spec- trum. Furthermore, AGNs physics is in the focus of astrophysicists also to establish the origin of Cosmic X ray Background.
III. Positron Astrophysics; positron production occurs in a variety of cosmic explosion and acceleration sites, and the observation of the characteristic 511 keV annihilation line provides a powerful tool to probe plasma composition, temperature, density and ionization de- gree. Compact objects, both galactic and extra-galactic, are be- lieved to release a signicant number of positrons.
IV. Establishing the precise role of non-thermal mechanisms in extended objects like galaxy clusters
V. Origin of cosmic hard X/soft g-ray diuse background VI. Physics of supernova explosions
For a detailed description of these issue see [Frontera and von Ballmoos, 2010], and the references therein.
In this perspective, Italian Space Agency funded the Laue project, with the aim to develop a new technology for building a Laue lens with a broad energy band (70 ÷ 300 keV) and long focal length (20 m), for astrophysics observations. This work is in part devoted to realize suitable optical elements, based on curved crystals, to be used as focusing elements in this lens (see Chap.
1.2 Medical application
On the basis of a know-how developed during the Laue project, another impor- tant project is funded by SPINNER (Emilia Romagna Region) with the aim of developing an innovative in-vivo medical imaging tool for tomography in nuclear medicine. This thesis is completely included in that project.
The term medical imaging indicates a group of techniques allowing to take images of inside of the human body (parts, tissues, or organs) for use in clinical diagnosis, treatment and disease monitoring; it certainly represented a revolu- tion in the world of medicine. Medical imaging shows a great versatility and it
nds so various applications.
It emerges the need to identify more advanced solutions in the eld of med- ical imaging technology with the goal to provide always more eective and high resolution images in order to achieve the most truthful diagnosis and accord- ingly making the best medical decision. This means not only the giving to patients of the best therapy, but also to avoid unnecessary procedures often caused by false positives or overestimated disease severity and prognosis.
Typically, the identication and monitoring of neoplastic diseases is per- formed by administering to the patient a specic radiopharmaceutical (biologi- cal compounds containing a radioactive isotope) to locate physiological abnor- malities in the body. These isotopes are typically g ray emitters of ∼ 100 ÷ 200 keV in energy and with half-lives T1/2on the order of a few hours (see Table 1.1).
The basic process for nuclear imaging involves introduction of a radiophar- maceutical into the patient (usually by intravenous injection) which subse- quently accumulates in the target site or biological process of interest. Higher concentrations of the radiopharmaceutical yield a higher g ray emission rate relative to surrounding tissues and background. These g rays are generally captured by means of gamma cameras that subsequently send the data to a computerized system that generates a two or three dimensional image (Adler et al., 2003) see (Figure 1.2.1).
Currently, most nuclear medicine imaging systems have limited spatial reso- lution that ranges from 7 to 15 mm [Roa et al., 2005]. For example the latest di-
Nuclide T1/2 g ray energy (keV) Purpose
Cr-51 28 d 320 red cell volume
Ga-67 79.2 h 93, 185, 300, 393 tumor location e inammation
I-123 13 h 159 imaging of thyroid
In-111 67 h 171, 245 labeling white blood cell
Tc-99m 6.02 h 140.5 Multi-purpose imaging
Tl-201 73 h 135, 166 Myocardial imaging
Xe-133 5.3 h 81 Ventilation imaging
F-18 1.83 h 511 Tumor imaging
Table 1.1: Typical radiopharmaceuticals used in nuclear diagnostic medicine.
Figure 1.2.1: Patient undergoing a scan using a gamma camera. Administration of a radiopharmaceutical (upper left display) [Roa et al., 2005] .
agnostic system in nuclear medicine, the Positron emitted Tomography (PET), can achieve resolutions of 4/5 mm at best. Furthermore, because the radio- pharmaceuticals needed for PET imaging have signicantly short half-lives (at most two hours), relatively large radiopharmaceutical doses must be prepared to leave enough activity to image the patient. In addition, most PET centers must be located in close proximity to a cyclotron facility, in order to minimize the transport time of the radiopharmaceutical from the preparation laboratory to the imaging room.
The possibility to obtain more dened, and therefore more accurate, images of the examined area depends on the ability of focusing radiations, and more precisely, of the lens interposed between the patient (g ray source) and the ra- diation detector. A Laue lens can increase, with respect to other diracting instruments, the focusing power. The application of this new system is envi-
sioned to scan the patient's body and, after a software elaboration, to produce 2D or 3D images with a spatial resolution of ≤ 2 mm. If a patient has under- gone a full-body scan and the data suggest the presence of a tumor or suspicious process (e.g., ischemia), a localized scan of that region could be performed with this imaging system without the need of injecting more radiopharmaceutical in the patient. This system may be better able to provide additional information to the size of the tumor or suspicious process and to dene its location more accurately .
The SPINNER project proposes to realize a new type of engineered Laue lens realized with curved crystals as optical elements. Curved crystals, in this case are not used as focusing optical elements, because the geometry of the lens is designed in order to focalize the incident X and g beam into a focal point.
Curved crystal are used to increase the angular acceptance of the lens and so to diract the most part of the photons that come from the radiopharmaceutical injected in the patient (Fig. 1.2.2).
Figure 1.2.2: Schematic diagram of a single lens constituted of curved crystals with its corresponding detector.
This method of g ray focusing and subsequent detection eliminates the need for high-spatial resolution collimators typically used in gamma cameras which causes signicant reduction in sensitivity (Chandra, 1999). Moreover, this pho- ton diraction imaging system can be tuned to diract a specic g ray energy (within∼ 100 − 200 keV) by simply adjusting the source-to-lens and lens-to- detector distance such that the lens remains equidistant between the source and detector. This adjustment changes the Bragg angle to match the dened g ray energy.
Diraction of X and g ray from crystals
In this chapter the theory of X and g ray diraction from real crystals is out- lined, starting from the simplest case: the kinematical theory from ideal crys- tals. Since for thick and real crystals this theory is limited, the dynamical theory of diraction is adopted. Dynamical theory allows to understand and to describe the diraction from mosaic and curved diracting planes (CDP) crystals, permitting also to predict their diraction eciency.
Basic and useful notions of crystallography are also introduced.
2.1 Fundamentals of crystallography
2.1.1 Crystalline structure
An ideal crystal is constituted by periodical repetition, in the three dimensions of the space, of a single or a group of atoms. The group of atoms constitutes the cell and it may have a very complex structure. The repetition of the cell can precisely cover the whole space, without superposition or vacancies, through innite translations. The primitive cell is the smallest cell that contains all the structural and symmetry informations to build-up the structure of the lattice by translations. The periodical repetition of the primitive cell is called Bravais lattice. It is built by three vectors not complanar and linearly independent a, b and c called primitive vectors; the primitive cell is the parallelepipedon, with volume Vc, dened by primitive vectors:
Vc= |a · b × c| (2.1.1)
The choice of these three vectors is not unique, so also the choice of the primi- tive cell is unlimited. A generic lattice vector t can be written as t= n1a + n2b + n3c
where n1, n2, n3 are integers.
The primitive cell and the Bravais lattice determine univocally and totally the structure of the crystal.
The classication of the crystal's structure is done by lattice translations and the symmetry operations, constituted by all rigid operations that convert the lattice in itself, leaving it unchanged . In three dimensions there are 14 Bravais lattices divided in 7 categories marked by given symmetry operations, Fig.2.1.1, .
Figure 2.1.1: The 14 Bravais lattices in the three dimensions. The a, b, and g are the angles between a, b and c respectively.
X-ray diraction from crystals is concerned with the scattering from atoms that may be thought as lying within families of planes called Miller indexes (h,k,l). For a given family of planes, the Miller indexes are dened such that plane closest to the origin (but not including the origin) with the intercepts (ha,bk,cl) on the axes (a, b, c) . The most important features of Miller indices are:
1. by convention, a negative intercept is represented by writing a bar over the correspondent Miller index;
2. the triplet hkl can be placed in parentheses, when it refers to a specic plane, and in accolades, when it refers to all crystallographic planes de- scribed by the same indices;
3. for a given family, the planes are equally spaced so it is possible to dene the distance dhkl between two sets of planes . In the simplest case of a cubic lattice, the d spacing is given by dhkl = √ a
h2+k2+l2 where a is the lattice parameter.
In Fig. 2.1.2 some examples of lattice planes in a cubic cell are represented.
Figure 2.1.2: Examples of lattice planes of a cubic cell.
2.1.2 Reciprocal lattice
In crystallography turn out to be useful consider another lattice called recip- rocal lattice. It is a pure mathematical concept (introduced by[Ewald, 1921]) that hasn't a physical meaning of a structural lattice, but it allows to represent more easily the crystallographic planes.
Starting from the direct lattice characterized by the primitive vectors (a,b,c), it is possible to built-up a lattice of imaginary points that have a precise rela- tion with the starting lattice. The basis of the reciprocal lattice is a triplet of vectors (a*,b*,c*):
a∗= b × c
Vc , b∗= c × a
Vc , c∗ = a × b
The relation that links the primitive vectors in real space with that ones in reciprocal space is deducible by eq 2.1.2:
a∗· a = 2π (2.1.3)
The volume of the primitive cell in reciprocal lattice is Vc∗ related with direct lattice by Vc· V∗c = 1. As in the real space, the distances between two sets of planes is d∗hkl and its value is d∗hkl= d1
2.1.3 Diraction condition: Bragg and Laue relation
The diraction depends on the crystal's structure and on the wavelength of the incident radiation, indeed when the wavelength is comparable with or smaller than the lattice parameters a diraction can occurs. Crystals are natural lattice diraction for X rays due to their periodic structure, with the periodicity of the order of the Angstrom. W. L. Bragg in 1912 gave an interpretation of the experiments on X ray diraction as the reection of the X rays on families of lattice planes and he formulated the Bragg's relations in 1913 (Bragg and Bragg, 1913).
The simplest approach to study X ray diraction from crystals is to treat it as an interference of rays scattered by a multitude of equidistant lattice planes.
The maximum of constructive interference occurs when the path dierence be- tween scattered waves is an integer multiple of the wavelength l. For an incident ray making an angle j with the scattering lattice planes spaced d, the dier- ence path between the incoming and the scattered ray is given by 2d sinj, see Fig 2.1.3. The formula to nd the maximum of the corresponding interference pattern known as Bragg's law is:
mλ = 2dhklsin θ (2.1.4)
where m has an integer value and it is known as the order of the correspond- ing reection.
Figure 2.1.3: In panel A: Bragg reection from a particular family of lattice planes, separated by distance d. The unit vectors s and s0represent the incident and diracted waves. The dierence path of diracted beam from two atoms is also shown
If a beam impinges on a crystal, each atom within the crystal can scatter the radiation in all directions. Diracted peaks are observed only in that di-
rections and wavelengths for which the scattered rays interfere constructively.
To nd this condition, two scatterers separated by a displacement vector d are considered, Fig.2.1.3 . The incident beam has a direction of propagation de- scribed by the unit vector s, a wavelength l and a wavevector k. A scattered ray will be observed in direction s0 with the same wavelength l of the incident beam and with wavevector k0, provided that the path dierence between the rays scattered by each atoms is an integral number of wavelengths.
From Figure 2.1.3 B the path dierence is d· (s − s0). The condition for constructive interference is that the path dierence is a multiple of l; expressing it in wavevectors:
d· k − k0 = 2πm. (2.1.5)
Because the reciprocal lattice is a Bravais lattice, if k and k' are reciprocal lattice vectors, so is (k − k0) = G(Laue condition), where G = ha∗+ kb∗+ lc∗is called scattering vector. It will be demonstrated that the Laue condition is equivalent to the Bragg relation expressed in eq. 2.1.4.
Assuming that the Laue condition is satised and that k and k' make an angle j with the planes perpendicular to G, see Fig. 2.1.4
Figure 2.1.4: Scheme of Laue condition. The scattering vector G is represented.
The distance between successive planes in a family must satisfy:
|G| = 2πm
and from the Fig. 2.1.4 is possible to obtain:
|G| =2|k| sin θ (2.1.7)
So from eq. 2.1.6 and eq. 2.1.7 and considering the denition of k as k = 2πλ , the Bragg condition nλ = 2d sin θ is found.
2.1.4 Ewald construction
PP. Ewald proposed in 1913 a simple and graphic construction, exhibited in Fig.
2.1.5 that may helps to visualize the diraction condition in three dimensions.
Draw a sphere in reciprocal space centered on the tip of the incident wavevec- tor k and with radius k (so that it passed through the origin). The wavevector k' satises the Laue condition if and only if a reciprocal lattice point lies on the sphere's surface and the directions of k' is the one joining the center of the sphere with the point on her. In this case there will be a Bragg reection from the family of real lattice planes perpendicular to that reciprocal lattice vectors.
Figure 2.1.5: The Ewald construction. The crosses represent the reciprocal lattice points of the crystal. Given the incident wavevector k and a sphere of radius k, diraction beam k' is produced whenever a reciprocal lattice point lies on the surface of the sphere.
The Ewald construction conrms that for a generic incident wave there will be no Bragg peaks. This constrain can be relaxed by the following experimental method:
1. Laue method. Fix the orientation of the single crystal and use a white X ray incident beam containing wavelengths from λ1 to λ0. The Ewald sphere is considered as the region contained between the two spheres de- termined by k and k0. The Bragg peaks will be observed corresponding to any reciprocal lattice vectors laying within this region.
2. Rotating crystal method. A monochromatic beam is xed in direction while the crystal rotates around the same xed axis. As the crystal ro- tates, the reciprocal lattice rotates by the same amount. Thus the Ewald sphere (which is determined by the xed incident vector k) is xed while the reciprocal lattice rotates around the axis of rotation of the crystal. For each reciprocal lattice point that traverses the circle during the rotation , the Bragg condition is satised and a diracted beam occurs.
2.1.5 Geometries of diraction
The X and g rays diraction from crystals can be realized in two dierent geometries: the Bragg geometry in which the reected beam rises from the same face in which the incident beam impinges, and the Laue geometry where the diracted beam comes from the opposite side of the crystal, in Fig 2.1.6 both geometries are represented. At high energies (E > 60 keV) the angle of diraction is very small (generally less than one degree), so to get diraction in Bragg geometry it's necessary a crystal with a large area. On the other hand the Laue geometry can be successfully adopted.
Figure 2.1.6: Laue and Bragg geometries. The lines inside of crystals represent the lattice planes. The angle θBsatises the Bragg relation
2.2 Diraction from ideal crystal
In this section the study of the diraction of X ray from a perfect crystal is presented, with an intuitive approach given by the geometrical diraction theory, called also kinematical theory.
2.2.1 Thomson scattering from a free electron
An electron of mass me and charge e is positioned on the origin of a coor- dinate system in which the x axes represents the propagation direction of an electromagnetic wave, with a wavevector k, that invests the charge. This wave is characterized by an electric eld E = E0e2πi(kx−νt), with E0 amplitude of the wave. The electron is supposed free and the eld exercises on it a force F = eE that produces a oscillation with an acceleration a = meEe and a fre- quency n, accordingly with that of electric eld. From the classical theory of electromagnetism, an electric charge accelerated emits radiation. Thomson has demonstrates that the eld produced by charge in a generic point Q at distance R from the origin of the axes is :
E(x, t) = − 1 4π0
R E0e2πi(kR−ν(t−Rc)−φ) (2.2.1) with:
y angle between the direction of the electron's acceleration and the direction of the observer,
φ the phase shift introduced by the process of re-injection of the wave by electron. It is possible to demonstrate that φ = π,
mec2 the length of diusion or classical electron radius re. It has a di- mension of a length. re ≈ 2.8179 10−15m.
It lies in the (x,y) planes as show in Fig. 2.2.1
Figure 2.2.1: Scheme of Thomson diusion. The electron is in the origin O of the reference system.
In terms of intensity:
sin ψ R E0
sin2ψ (2.2.2) with I0value of incident intensity. This intensity Ip is inversely proportional to the square of the mass of the electron. This means that the particles heavier than it, as example the proton, contribute at the intensity 18372times less that the electron.
Suppose now that the incident beam is polarized:
along z axes: Ip = I0 1 4π0
along y axes: Ip= I0 1 4π0
cos22θ with 2θ the angle between the in- cident beam and the direction of observation.
In general is necessary to decompose the incident beam in two components, one parallel and the other one perpendicular to the plane that belongs the direct beam and the direction of observation. In this case the intensity Ip becomes:
Ip = I0re R
where P is called polarization factor and it's value is:
σ−polarization π−polarization random polarization
In the diraction from hard X and g rays, the diraction involves very small angles, generally less that one degree. So the value of the three polarizations can be assumed as ≈ 1 and in term of intensity this parameter can be neglected.
The Thomson scattering is a coherent scattering because there is a precise relation between the frequency of incident and diuse beam.
2.2.2 Scattering from an atom
Classical scattering from a group of electrons conned to a small volume are discussed (Warren, 1969) and a scheme is represented in Fig. 2.2.2 A. The incident beam, of amplitude E0, has a propagation direction represented by the unit vector s. The electrons n are distributed around point O at r position.
The scattering are studied in point Q at a large distance R from the electrons in a direction given by a unit vector s'.
Figure 2.2.2: Panel A: Scattering from a group of electron at distance r from the origin.
The point Q is the point of observation. Panel B: relation between the vector of the incident s and scattered direction s' with vector position r
The value of the incident electric eld in point Q is given by E = E0
2πνt − 2π
λ (D1+ D2)
Considering that the distance of the source and the R are both very big com- pared to r, it is possible to write D2 as R and:
D1+ D2= R − (s − s0)·r =R − ∆S · r
Expressed in terms of the complex exponential, the diuse electric eld at distance R is the sum over the electron n:
E = E0re
e2πi/λ∆S·r (2.2.5) To calculate the coherent scattering from an atom, each electron can be considered spread out into a diuse cloud of negative charge, characterized by a charge density r(r). The quantity r(r)dr is the ratio of the charge in volume dr centered on r position, so that for each electron
ρ(r)dr = 1. The wave mechanical treatment says that the amplitude of scattering from the element r(r)dr is equal to rdr times the amplitude of classical scattering from a single electron. The total amplitude of scattering is calculated considering that instead of electrons at positions r, we have charge elements pdV at positions r, and by replacing the sum by an integral the eq. 2.2.5 can be written as:
E = E0re
e2πi/λ∆S·rρ(r)dr (2.2.6) The integral
e2πi/λ∆S·rρ(r)dr = feis called the scattering factor per electron and it represents the scattering amplitude per electron, expressed in electron units. Assuming a spherical symmetry for the charge distribution r(r), the terms ∆S·r can be written in polar coordinates as 2r sin θ cos φ (see Fig.2.2.2B) and with the abbreviation k =4π sin θ/λthe fecan be simplied as:
eikrcosφρ(r)2πr2sin φdφdr (2.2.7) The integration with respect to φ is readily performed, so
2πr2ρ(r)sin kr kr dr
As the same for electric eld, the intensity of the scattering per atom f is the sum of the intensities of the scattering from the electrons:
2.2.3 Diracted intensity from a small single crystal
Based on the Thomson scattering described above, the scattering from a more complicated objects such as crystals is now considered. The details of this study is developed by many authors from which Warren (Warren, 1969).
A monochromatic beam, of intensity I0, wavelength l, and with a direction represented by the unit vector s, falls on a small crystal. The crystal is at the origin O and the position of the atoms m in unit cell n1n2n3 are given by Rmn = n1a + n2b + n3c + rm. The intensity of the scattering from the crystal is studied at a generic point of observation Q, in a direction specied by a unit vector s' and at a distance R. The conditions are very similar to that illustrated in Fig. 2.2.2 where r can be substituted by Rmn . Following the treatment of par. 2.2.2 , the instantaneous value of the electric eld at the point Q from the atom (m, n) is given by
E = E0
Rfmei2πνt−(2πiλ )[R−∆S·(n1a+n2b+n3c+rm)] (2.2.9) The total value of electric eld at Q is due to all the atoms in the crystal, so it is obtained by summing over m to include all the atoms in a unit cell, and summing over n1n2n3 to include all the unit cells. It is possible to approximate the crystal as a parallelepipedon with N1number of cells along the axis a, N2
along the axis b and N3 along c so that N1N2N3 = N is the number of unit cells in the crystal. Separating the summations, the instantaneous eld in Q is expressed by
E = E0re
e2πiλ ∆S·(n1a+n2b+n3c) (2.2.10)
The summation over m involves the positions rm of the dierent atoms in the unit cell and it varies from one structure to another. It is called the structure factor F and it is dened as:
fme2πiλ∆S·rm (2.2.11) The quantity Fhkl plays an important role in the diraction theory. If
∆S = 0, the structure factor F is simplyF = Pmfm, so F approaches the atomic number Z. This means that the structure factor gives immediately an estimation of the number of scatters in the atom.
The summations over n1, n2, n3 in eq. 2.2.10 have the form of geometric progressions and they can be rewritten as: e2πiλ ∆S·N1a−1
So the value of the electric eld in Q is:
E = E0re
Rei(2πνt−2πλ)Fhkle2πiλ ∆S·N1a− 1
e2πiλ ∆S·a− 1 ×e2πiλ ∆S·N2b− 1
e2πiλ ∆S·b− 1 × e2πiλ ∆S·N3c− 1 e2πiλ ∆S·c− 1
(2.2.12) To nd the intensity of the electric eld Ip in Q it is required to calculate EE∗ and express it in a simplest form. In particular it is possible to develop the three exponential expression in a geometrical form:
eiNx− 1 eix− 1
e−iNx− 1 e −ix−1
= sin2 Nx2
So the intensity of the electric eld is:
PF2hklsin2 πλ ∆S · N1a
sin2 πλ ∆S · a ×sin2 πλ ∆S · N2b
sin2 πλ ∆S · b ×sin2 πλ ∆S · N3c sin2 πλ ∆S · c
(2.2.14) The three equations y = sinsin22Nxx called Laue equation determine the intensity.
The function y is essentially zero everywhere except in proximity of x = nπ, where the function reaches the maximum value. So the diracted intensity Ip
is essentially zero while it can achieve a maximum when the three quotients are simultaneously close to zero:
∆S · a = hλ
∆S · b = kλ
∆S · c = lλ
These three equations together are equivalent to the Bragg law.
18.104.22.168 Integrated intensity from small single crystal
The most useful quantity which can be both calculated and measured is the
"integrated intensity" and which gives directly information of the diraction eciency of the measured crystal.
Lets consider a collimated incident beam impinging on a small single crystal at the Bragg angle θB for the set of planes (hkl). The diracted beam falls normally upon a receiving surface at distance R from the crystal where it is detected.
Since intensity is energy per unit area per unit time, the integrated intensity Iiis the total energy obtained by integrating Ipover time and over the area of the detector. It is convenient to represent the three Laue conditions in eq. 2.2.15 as a vector in reciprocal space ∆S · c = lλ = λ (p1b1+ p2b2+ p3b3)with b1b2b3 reciprocal vectors and p1p2p3 integer coecients. So the value Ii in a volume in the reciprocal space dV = sin 2θdαdβdγ becomes:
Ii= Ip R2 sin 2θF2hkl
sin2π · N1p1 sin2πp1
sin2π · N2p2 sin2πp2
sin2π · N3p3
sin2πp3 dV (2.2.16) Developing the three integral in all reciprocal space and reminding that N1N2N3= N , the nal expression for the total integrated energy can be ob- tained:
Ii= I0 r2eλ3V
Vcsin 2θF2hklP (2.2.17) where V is the volume of the small crystal and Vc is the volume of the unit cell.
Introducing a parameter L as Λ = reλ|FπVchkl| called extinction length the Iican be written as:
π2λ Λ2sin 2θ
cos θP (2.2.18)
where the volume of the crystal crossed by the beam can be considered as the thickness t divided by cos θ. The subscript kin helps to remind that this results is valid for the kinematical theory
Is possible introduce the integrated reectivity Ri,kin as the ratio between integrated intensity and the incident intensity:
Ri,kin = Ii,kin
This treatment is true for a non absorbing crystal while for absorbing crystal the eq. 2.2.18 becomes:
Ri,kin = π2λ Λ2sin 2θ
cos θPe−cos θµt (2.2.20) 2.2.4 Limitations and corrections to the kinematical theory:
the dynamical theory
As previously said, the kinematical diraction theory is not the correct treat- ment for a complete and exhaustive description of diraction by crystals. Indeed it is based on some approximations:
1. the interference between incident and diracted beam is not considered, as also the interference that occurs between the scattered beams from crystals (multiple scattering),
2. the thickness of the crystal is small enough to consider the absorption negligible,
3. the refraction index of the crystal is very close to the refraction index of the environment. This assumption is always valid for X and g rays.
4. The principle of energy conservation is violated: in eq. 2.2.18 the inte- grated intensity diracted by a crystal is proportional to its thickness, so the integrated intensity tends to innity when the thickness goes to inn- ity. This happens because the diusive centers in deeper layers receive an incident beam that is considered with the same amplitude of that received in the surface layers. This ignores the interaction of the wave with matter.
Darwin (Darwin, 1914) was the rst to mark the kinematical theory as incorrect.
He introduces the concept of the waveeld: he describes the incident electric
eld that propagates in the crystal as a sum of plane waves with wavevector that diers from each other by a reciprocal lattice (Bloch waves). The aim of this theory is to determine the possible positions for the tiepoint and so to describe the waveeld that propagates in the crystal. It will be shown that the results of the dynamical theory tend asymptotically to those of the kinematical theory when the crystal thickness is much smaller that a quantity dened by the extinction length, that is inversely proportional to the structure factor Fhkl
and to the wavelength l.
In this thesis the details of the dynamical theory will not be investigated because of their complexity, but the most important results will be exposed, to better understand the problem to obtain crystals for a Laue lens. The reader can nd a much more complete treatment of the dynamical theory in Authier (Authier et al., 1996)
2.2.5 The dispersion surface
Is possible to represent this concept starting from the Ewald construction. Fig.
2.2.3 shows how one passes from the Ewald sphere to the representation of the Bragg condition. The Laue point La is the center of the Ewald sphere, it is situated on the intersection of the two spheres centered at the reciprocal lattice nodes O and H with a radius of curvature k = 1λ; the position of Laexactly satises the Bragg condition.
The waves propagating in the medium interact with matter characterized by an index of refraction n. For X and g rays this index is slightly less that one so the wave number of waves propagating in the crystal is nk < k and another two spheres of radius nk can be drawn inside the other ones; now the point representing the Bragg condition is on the intersection of the two spheres, called Lorentz point Lo, see Fig. 2.2.4 . The distance between the Lorentz and the Laue point is LoLa=k(1−n)/cosθb. The wave propagating in the incident direction is called refracted wave.
Figure 2.2.3: Diraction condition according to the kinematical theory from a recip- rocal space. −→
OHis a vector of reciprocal space, La is the Laue point that satises the Bragg condition, OLa= k0and HLa= khare the wavevector of incident and reected beam respectively, (kOLak = kHLak = 1/λ). OM is a wavevector that don't satises the Bragg's condition. Both the dotted spheres have a radius of k.
Contrary to kinematical theory, in a semi-innite crystal (ideal case) the re-
ection can occur for an angular range in which the Bragg condition is satised, called reection domain. So, for every position within the reection domain, there is a refracted beam, of wavevector k0 = OPcoexisting with the reected wave kh= HP, Fig. 2.2.5. For reason of symmetry, P don't lie on either of the two sphere but on a connecting surface between them, called the dispersion sur- face. In this case there are two coexing waves, with wavenumbers diering from nk and closely linked to form a waveeld; to stress this concept Ewald called the point P tiepoint. The position of P determines the direction of propagation of the waveeld.
The angular width of the reection domain is represented in reciprocal space by the size of the dispersion surface, which diameter is proportional to Fhkl. So the larger is the structure factor, so is the reection domain and the stronger is the interaction. The dispersion surface is constituted by two hyperbolae in the proximity of Lo, with a distance from it given by the inverse of the extinction length, indeed the distance of Lorentz point to the dispersion surface is shorter than the distance of the Lorentz point to the Laue point.
22.214.171.124 Qualitative approach to the dynamical theory
The wavenumber of the wave propagating in the vacuum in the incident or reected direction is k and the common extremity M of their wavevector OM = k0 and HM = kh lies on the sphere of radius k and centered in O and H
Figure 2.2.4: Inuence of the index refraction on the Ewald construction. The Bragg's condition is now satised in the the Lorentz point Lo that lies in the intersection of the spheres of radius nk (solid line). The vector OP is the refracted wave and HP the reected wave.
respectively, passing through the Laue point La. The intersections of these spheres with the plane of incidence are two circles which can be approximated by their tangent T00and T0h , and the distance LaM is k∆θ where ∆θ is the angle between OM and the direction that satises the Bragg condition. In the crystal, the incident wave OM excites two waveelds, characterized by the tiepoints P1 and P2 that are the projections of M on the two branches of the dispersion surface along the normal of the surface of the crystal, see Fig. 2.2.6 .
In the crystal the waveeld propagates on straight line parallel with the Poynting's vectors S1 and S2, respectively normal to the dispersion surface in P1and P2 and symmetric with respect to the diracting planes. The Poynting's vectors are proportional to
Si ∝ E20+ E2h = s0|E0|2+ sh|Eh|2
where E0and Ehare the amplitudes of the waves that constituted the wave-
eld i, and s0 and sh are respectively the unit vectors indicating the incident and reected directions.
The separation of the intensity between waveeld i at the entrance surface results from boundary conditions applied to the electric eld vectors. The in- tensity is higher in the waveeld with Poynting vector closer to s0 and the ratio of the two waveeld intensities increases with increasing the angle between the Poynting vector and the reecting planes. At the exit surface of the crystal, the waveeld splits into a reected and a transmitted wave. Their intensities are again given through boundary conditions and one nds that the as Poynt- ing vector is closer to sh the reected intensity is higher (or inversely if the
Figure 2.2.5: Representation of the refracted OP and reected wave HP that are coexisting. The surface dispersion (solid line) is the surface that connect the two sphere and P is the tiepoint.
Poynting's vector is much closer to s0 the transmitted intensity is higher).
When the crystal rotates, the point M moves along the tangent T0 and crosses the Laue point, which corresponds to the exact Bragg condition. The tiepoints P1 and P2 move along the dispersion surface through its center. For an incident wave far from the Bragg condition, the Poynting vectors S1 and S2 are almost parallel to s0 and sh on one side of the Bragg peak, and to sh
and s0on the other side. In both cases, all the intensity is transferred to the waveeld parallel to s0 , the Poynting vector is parallel to s0 and at the exit surface there is only a transmitted wave. This is expected since, far from Bragg incidence, the beam passes straight through the crystal that is only aected by normal absorption (Keitel et al., 1997).
Some important parameters can be deduced by the geometrical construction of the dispersion surface, and they can help to express the reectivity and the integrated intensity in the dynamical theory.
The asymmetry ratio: Let γ0= cos ψ −θBand γh = cos ψ +θB be the cosine of the angles between the normal to the surface of the crystal and the incident and reected beam (y is called asymmetry angle), respectively. Their ratio γ is so dened:
γ = γ0
γh = cos (ψ − θB)
cos (ψ + θB) (2.2.21)
The Darwin width δw is the full width at half maximum (FWHM) of the rocking curve in the Laue geometry and the width of the total reection domain in the Bragg geometry. It is expressed by:
δw= dhkl Λ = λ
sin 2θB (2.2.22)
Figure 2.2.6: Scheme of the dispersion surface and of the boundary conditions in the Laue geometry. O is the origin of reciprocal lattice and OH is a reciprocal vector. s0
and share respectively the unit vector of the incident and reected directions. MO is a wavevector of the incident wave, La and Lothe Laue and Lorentz points. S1and S2
are the Poynting' vector and P1 and P2 the tiepoint on the dispersion surface. T00 is the tangent of the circle of radius k, T0and Th are the tangent of the circle of radius nk centered in O and H respectively [Authier et al., 1996]
where L is the Pendellösung distance in the Laue geometry and the extinc- tion length in the Bragg geometry dened in par. 126.96.36.199.
The deviation parameter h in the Laue geometry is:
η = ∆θ
where ∆θ is the deviation from the exact Bragg condition.
2.2.6 Integrated Intensity and reectivity in Laue case in dy- namical theory
The integrated intensity Iiis the area under the diraction prole. In dynamical theory the expression for the integrated reectivity by a non absorbing crystal is:
Ri,dyn = π2P 2 sin 2θB
where A = πtΛ , B0(2A) =2A
0 J0(z) dz and J0(z) is the Bessel function of 0 order.
The Fig. 2.2.7 represents the variation of B0(2A) as a function of the thickness t/Λ. The value oscillates around 1 when the thickness of the crystal increases and becomes 1 when the thickness goes to innite. This oscillation, called Pendellösung eect is due to the interference of the refracted and reected waves [Halloin and Bastie, 2005]. The periodicity of the oscillation is the same of the extinction length, with a minimum in correspondence of it. If the crystal is absorbing the oscillation is quickly smoothed .
Figure 2.2.7: Variations of the integrated reectivity with the thickness in case of absorbing non absorbing crystals.
When A tends to 0, i.e. t Λ, the function B0(2A)tends to 2A. In this condition one can nd that:
So this mean that the kynematical theory can be considered the limit of the dynamical theory for small crystals. The transition between the two theory is leaded by the extinction length. When t Λ the kinematical theory can be applied whereas t Λ the crystal is thick and the dynamical theory can be adopted.
On the basis of the dynamical theory, W. H. Zachariasen (Zachariasen, 1945) presents the theory in a form which enables a direct quantitative comparison with experiment. It is possible to calculate the intensity of reection and trans- mission of a parallel monochromatic X ray beam as a function of the angle of incidence to the reecting planes. The reectivity R and the transmittivity T are obtained from the ratio of the diracted and transmitted beam respectively with the incident one (Hirsch, 1951) :